AN INSIDE LOOK AT CORROSION IN COmpOSIte · PDF file 2010. 10. 4. · ASTM C581...
Embed Size (px)
Transcript of AN INSIDE LOOK AT CORROSION IN COmpOSIte · PDF file 2010. 10. 4. · ASTM C581...
AN INSIDE LOOK AT CORROSION IN COmpOSIte LAmINAteS
Boron-Free e-CR Glass Fibers Demonstrate Superior Corrosion Resistance Compared to e-Glass When Used in Composite Structures exposed to Sulfuric Acid. previous Research on Leaching mechanism of e-Glass in Acids is Confirmed Visually.
By Kevin Spoo, CCt, CCt-C, 6σ Research Associate, OCV™ Reinforcements, and marie Kalinowski, Senior Scientist, Owens Corning Analytical testing and terry Gano, Research technician
Abstract The superior corrosion performance of boron-free Advantex® E-CR glass compared to E-glass has been shown in many ways. Numerous bare-glass corrosion studies have compared various glass compositions but do not necessarily reflect composite corrosion performance. ASTM C581 composite corrosion performance testing shows composite performance in a “no-stress” testing methodology and thus is really a resin test rather than a test of a composite system under load. Stress-corrosion work started by Mark Greenwood at Owens Corning in the mid-1990s and continued at the company tests composites under load and provides a compelling reason for using superior glass reinforcement (Advantex® E-CR glass) throughout the structure. The mechanism for the corrosion of E-glass has been inferred through previous leaching studies. This paper shows E-glass deterioration visually and the mechanism by which it occurs.
Introduction There are a number of ways in which the corrosion of E-glass has been studied relative to other glass fiber products. A comparison of bare-glass corrosion in various corrosive media is the simplest. But it is an incomplete way of understanding what happens in the
composite part. A comparison of glass fibers in ASTM C-581 coupons can show differences between E-glass and Advantex® E-CR glass, but the test was originally designed to compare the performance of
corrosion resistant resins in a no-load condition. Any differences between E and E-CR glass in an ASTM C-581 must be very large to show a difference. Mark Greenwood’s stress- corrosion work started in the mid-1990s and continued today by Kevin Spoo combines both corrosion and stress to predict the relative performance of E-glass compared to Advantex® glass under these dual conditions. The focus of this paper is to show the mechanism by which corrosion occurs over time in stressed laminates using SEM (Scanning Electron Microscopy) and EDX (Energy Dispersive X-ray) spectrometry.
The focus of this paper is to show the mechanism by which corrosion occurs over time in stressed laminates.
Corrosion of Glass Fibers Most composite materials intended for corrosion resistant applications are designed to protect the structural fibers within the architecture of the part. This paper is not going to delve into that, but instead focus on what happens as corrosive materials gain access to the structural portion of a laminate.
What we think happens, and numerous publications support this view, is that corrosive materials gain access to glass fibers through the protective coatings or resin matrix. Quality coatings or resin matrices can slow corrosion by addressing the several mechanisms by which corrosive materials gain access to the glass fibers. These mechanisms include access through cracks in the resin matrix created as a result of: 1) matrix shrinkage, 2) applied stress or strain as part of the design, 3) environmental cycling (which is really a stress or strain), or 4) damage through impact (which is another stress or strain).
Other mechanisms which do not rely on cracks are: 5) process upset exposing resin matrix to more corrosive materials than were intended, 6) poor resin matrix selection and 7) diffusion of the corrosive material through the intact resin matrix. The effect of diffusion is highly dependent on the corrosive media and the resin matrix. Previous studies have gathered data to quantify the effect of corrosion on the glass fibers. In this study, we attempt to actually see (visually) the corrosion progress over time.
testing process This study focused on the corrosion of glass fiber-reinforced composite rods that were exposed to a ~1% strain for a brief period of time and then immersed in a 10% sulfuric acid solution under no-load and room temperature for an extended period of time. After regular intervals the rods were removed and examined for the effects of corrosion.
This experiment used 17u E-glass and Advantex® glass fibers with the same identical sizing system and resin system to make pultruded rods. In order to ensure that the strain induced in the production of the rods was minimized, the glass fibers for making the rods were pulled by hand and not using a pultrusion machine.
Skeins of glass fiber were weighed, pulled through a resin bath and into hollow glass rods. The rods were then cured in an oven to ensure full and complete cure of the resin system. The resin system in this case was an isophthalic-acid-based unsaturated polyester resin at 400cps initiated with 1% BPO pre-dissolved in styrene.
After curing, the glass tubes were lightly rapped to shatter them and the hand-pulled pultruded rods were removed. Tabs consisting of steel tubing were bonded to the sanded rod ends using epoxy resin. The tabbed rods were placed in an Instron® tester and the breaking strength of the rods determined. A cantilever beam frame (see photos below) was then loaded with a load cell in place such that a 1% strain would be induced in the rod when placed in the fixture. The frame was unloaded, the load cell removed, the rod placed in the frame and the rod loaded to 1% strain. The rod remained in place for 72 hours.
Corrosive materials gain access to glass fibers through the protective coatings or resin matrix.
When the rod was removed, it was cut into 2” long pieces and immersed in a 10% sulfuric acid solution. It remained is this solution at 25ºC for several months. Rod pieces were removed periodically and examined by the Owens Corning Microscopy Lab. Unlike the photo on the far right shown below, these rods were not exposed to corrosive fluid under stress as is typical in stress-corrosion testing.
The preparation procedure used in the Microscopy Lab was to pot the sample in epoxy resin and remove about 1mm of material from the rod end through polishing of the sample. SEM photos were taken of the rod cross-sections at various levels of magnification. Additionally, when corrosion of fibers was seen, EDX spectrographs were made to determine if corrosion was actually taking place by monitoring compositional changes in areas of the glass fiber.
Findings and Discussion The SEM photos below were taken in back-scatter mode. An interesting feature of SEM is that electrons scattered from the surface of the part being examined will reflect a greater number of electrons from harder surfaces, such as solid glass fibers. Softer or porous surfaces like resin will reflect fewer electrons and voids reflect nothing. In SEM photographs, solid glass appears white or light gray, porous glass appears gray, resin appears dark gray and voids are black.
1. E-glass rod, one month in 10% H2SO4
2. Advantex® glass rod, one month in 10% H2SO4
Photos 1 and 2 show low magnification views of the E-glass and Advantex® glass samples after one month exposure to 10% sulfuric acid. The photos serve as a reference of the corrosion resistance of each glass type before examining selected areas of the rods. They also serve as a reference when comparing the differences between one-month exposure and three-month exposure.
When looking at the 1/8” E-glass rod in cross-section (photo 3), what we see is white fibers near the center of the rod, gray fibers at the exterior of the rod and voids apparent along the crack. The gray fibers have had components of the glass leached from the fiber. This proceeds from the outside of the rod inward and from the outside of the individual filaments inward.
A de-bonding of a number of fibers from the resin matrix has also occurred. The task of polishing the surface to obtain these photomicrographs could be suspected of creating these cracks, but normally if that had occurred cracks would be dispersed throughout the circumference of the part, and they are not. The rods were under no stress during chemical exposure, so a likely cause could be latent resin shrinkage as the resin de-bonds from the fiber and the fiber disappears.
This resin, like most unsaturated polyesters, has an 8% volumetric shrinkage and latent built-up stress is possible. The task of polishing accounts for some of the fibers being pulled out of what is now a void area. The empty holes where fibers were previously, appears black (void).
Confirmation of leaching was obtained by running EDX spectrometry on fibers in photos 4 and 5 with the locations of each sampling appearing with green numbers on the sampling locations. EDX is a fast and convenient tool for measuring the composition of glass fibers but it does have some drawbacks. It cannot measure elements of atomic weight lower than carbon (C), and this includes boron (B). Boron is a key element in E-glass and previous studies have shown it is attacked readily by acids.
In fact, previous studies have shown the presence of boron dramatically increases the leaching rate of E-glass until only a silicate structure is left. An internal study at Owens Corning in 1986 identified boron as the ingredient that caus